Brill made various trips to the Middle East, including accompanying Theodore Wertimes 1968 survey of the ancient technologies of Iran, alongside other great minds such as the noted ceramicist, Frederick Matson (UCL Institute for Archaeo-Metallurgical Studies 2007). In the years 1963-1964, the Corning Museum of Glass and the University of Missouri, following a long history of excavation at the necropolis of Beth SheArim, conducted an examination of a huge slab of glass, some 2000 years old, that had been languishing in an ancient cistern (Brill and Wosinski 1965). Brill cannot recall who first suggested this slab, measuring 3.4m by 1.94m, could be made of glass, but the only way to test it was to drill a core through its 45 cm thickness and analyse it (Brill 1967, Brill and Wosinski 1965). On analysis of the core, Brill found that the glass was devitrified and stained, and not very homogenous, with a presence of wollastonite crystals throughout (1965, 219.2). Investigation of the manufacture technology required to produce the slab, suggested that in order to produce such a slab of glass, it would have been necessary to heat over eleven tons of batch material, and sustain it at around 1050˚C for between five and ten days (Brill 1967)! His initial interpretation was that the glass must have been heated either from above or from the sides using a kind of tank furnace; a hypothesis that was proven accurate when excavation underneath the slab suggested it had been melted in situ, in a tank whose floor was a bed of limestone blocks with a thin parting layer of clay (Brill and Wosinski 1965, Brill 1967). Brill's interpretation, that the slab and its surroundings suggest ‘some early form of reverberatory furnace’ was the first suggestion of the use of tank furnaces in early glassmaking (1967, 92). The evidence at Beth She’arim encouraged further innovative thought because whilst the slab represented glass production on a grand scale, no associated evidence for glass working was found. Brill had already suspected that historical glassmaking occurred in two phases, the heavy ‘engineering’ stage when the glass is formed from the batch ingredients and the ‘crafting’ stage when the glass is formed into artefacts (Brill, pers. comm., 2009). These stages could occur in combination at one location, or at two differing locales, and the time span of production after the initial glass melt is highly flexible. For Brill, the idea of this ‘dual nature of all glassmaking’ was ‘crystallized’ at Beth She’Arim, where only the raw glass production was represented, and would be reinforced later by the contrasting evidence, where working was favoured over production, found at Jalame, as discussed below (Brill, pers. comm., 2009).